# Interpreting finite element results for brittle materials in endodontic restorations

- Antonio Pérez-González†
^{1}Email author, - José L Iserte-Vilar†
^{1}and - Carmen González-Lluch†
^{1}

**10**:44

**DOI: **10.1186/1475-925X-10-44

© Pérez-González et al; licensee BioMed Central Ltd. 2011

**Received: **2 December 2010

**Accepted: **2 June 2011

**Published: **2 June 2011

## Abstract

### Background

Finite element simulation has been used in last years for analysing the biomechanical performance of post-core restorations in endodontics, but results of these simulations have been interpreted in most of the works using von Mises stress criterion. However, the validity of this failure criterion for brittle materials, which are present in these restorations, is questionable. The objective of the paper is to analyse how finite element results for brittle materials of endodontic restorations should be interpreted to obtain correct conclusions about the possible failure in the restoration.

### Methods

Different failure criteria (Von Mises, Rankine, Coulomb-Mohr, Modified Mohr and Christensen) and material strength data (diametral tensile strength and flexural strength) were considered in the study. Three finite element models (FEM) were developed to simulate an endodontic restoration and two typical material tests: diametral tensile test and flexural test.

### Results

Results showed that the Christensen criterion predicts similar results as the Von Mises criterion for ductile components, while it predicts similar results to all other criteria for brittle components. The different criteria predict different failure points for the diametral tensile test, all of them under multi-axial stress states. All criteria except Von Mises predict failure for flexural test at the same point of the specimen, with this point under uniaxial tensile stress.

### Conclusions

From the results it is concluded that the Christensen criterion is recommended for FEM result interpretation in endodontic restorations and that the flexural test is recommended to estimate tensile strength instead of the diametral tensile test.

## Background

Advances in endodontic restoration in dentistry have generalized the use of prefabricated posts for restoring devitalized teeth, especially when the coronal tooth structure is severely damaged [1]. The artificial post connects to the core over which is placed the restored crown, helping the transmission of the dental loads from the coronal structure to the root.

In recent decades, finite element (FE) simulation has been increasingly employed for analysing the biomechanics of the post-core endodontic restorations [2–13]. FE simulation has the advantage that random variability is avoided, unlike experimental in vitro tests. Moreover, the results obtained from a finite element model (FEM) of the restored system contain information about the stress distribution of each component of the restoration, instead of only a single value of failure load typical of in vitro results.

A correct interpretation of FEM results should be based on the stresses and strength of each component in the system. To obtain accurate conclusions from this interpretation, three conditions must be fulfilled: first, stress values must be reliable, i.e., the FEM should adequately represent the real system; second, strengths of the different materials present in the model must be known; third, an adequate failure criterion must be used to compare values of computed stresses, which are bi-axial or tri-axial, with material strengths frequently obtained under conditions of uniaxial stress state (tension or compression). The first condition is progressively approached with three-dimensional models, with finer meshes and more components represented in the system, although a good representation of bonded interfaces is difficult due to its small thickness. Moreover, some uncertainty exists about some of the material elastic properties. In addition, for most models all materials are considered to have linear isotropic behaviour, though this is a simplification for components such as dentine or fibre posts. However, the second and third conditions are not met in most previous work: the second due to the lack of consistent and complete data about the strength of some dental materials; the third due to the absence of a post-hoc analysis of failure in each component of the FEM or the use of the Von Mises equivalent stress as the reference value for this analysis. It is known that the Von Mises criterion is only valid for ductile materials with equal compressive and tensile strength [14], but materials exhibiting brittle behaviour such as ceramics, cements or resin composites are used frequently is these restorations. Even dentine presents reported values of compressive strength significantly greater than tensile strength [15].

Little research has been devoted to the interpretation of FEM results in post-core restorations. Most previous work has analysed the results of FE simulations from Von Mises maximal stresses [4–6, 8, 9, 11–13, 16]. The prevalent use of the Von Mises criterion is probably associated to the fact that this is the normal criterion for most engineering analyses, which usually deal with ductile materials such as steel or aluminium. All the commercial FE programs include this criterion as one of the default outputs in their post-processing modules. Moreover, this criterion makes it possible to talk in terms of an equivalent Von Mises stress, which is directly comparable to tensile strength and is thus a nice, simple failure criterion. For brittle materials, however, it is not possible to obtain an equivalent stress from the stress tensor, regardless of the material strengths, so that it can be compared with a strength value, because the compressive strength is normally different and greater than the tensile strength. To make up for this, some authors suggest the use of the Rankine or Maximum Normal Stress criterion to evaluate the failure in dentine, using the maximum principal stress to analyse the results [17, 18]. Others analyse results of shear stress in the post-dentine interface, indicating that this value should be compared to the reported shear bond strengths to evaluate the risk losing retention [4, 5]. Dejak et al. [19] applied the Tsai-Wu criterion for anisotropic materials to dentine, enamel and resin composites in molars with ceramic inlays. DeGroot et al. [14] compared three criteria to analyse FEM results in composite resin: Von Mises, a modified Von Mises criterion presented by Williams [20], and the Drüker-Prager criterion, concluding that Drüker-Prager is more suitable to describe the failure of this material. Recently, Christensen [21] proposed a unified failure criterion for ductile and brittle materials, which is equivalent to the modified Von Mises criterion proposed by Williams with an additional modification for brittle materials, and demonstrated some unrealistic behaviour of the Drüker-Prager and Coulomb-Mohr criteria under some important stress states.

Regardless of the failure criterion, reliable information about compressive and tensile strengths is needed for each material in the restoration. The compressive strength is usually obtained experimentally by a compressive test using cylindrical specimens. Tensile strength is obtained by applying an axial pulling force over specimens with a cylindrical or rectangular cross section and is a typical test for metals and other ductile materials. This type of test, however, is rarely used for brittle materials. Technical problems related with gripping and aligning the brittle specimens are often cited as an explanation for not measuring the tensile strengths [22, 23]. Alternatively, the diametral tensile test (DTT) is commonly used to obtain a diametral tensile strength (DTS) [23–26] because of its simplicity and reproducibility [27]. The DTT is performed by compressing a cylindrical specimen with its axis being perpendicular to the load direction. Tensile strength can also be obtained indirectly as a flexural strength (FS) with three or four point flexural tests (FT) [23, 25]. However, DTS and FS are obtained in loading states that are not uniaxial and the results of these tests are not equivalent, as numerous previous works have shown for different dental materials [22, 23, 25, 28, 29]. Despite this, DTS and FS, have been used interchangeably in recent works as a reference to compare to computed maximal stresses in finite element models of dental restorations [30, 31].

The objective of this paper is to discuss the problem of interpreting finite element results of the simulation of dental restorations and to propose some rules to do this interpretation correctly, with special attention to the failure criteria in brittle components. Additionally, the relationship between DTS and FS is analysed and the procedure for the correct use of these values for the failure criteria of brittle materials is discussed.

## Methods

Different failure theories employed in mechanical analyses were compared in this study to determine how suitable they were for use during the interpretation of FE results in dental restorations. These theories were: Von Mises (VM), Rankine (R), Coulomb-Mohr (CM), Modified Mohr (MM) and Christensen (C). All of these theories combine principal stresses at a point in a solid (*σ*
_{1}, *σ*
_{2}, *σ*
_{3}) with the compressive strength (CS) and tensile strength (TS) of the material to obtain a safety factor (SF) at this point. Safety factor values lower than unity indicate that the material is prone to have a mechanical failure at this point, and values greater than unity indicate a safe condition at this point. All of these criteria are used in mechanical engineering texts [32], except the Christensen criterion, which has only been recently presented in the literature [21]. These criteria are formulated below, with *σ*
_{1} ≥ *σ*
_{2} ≥ *σ*
_{3} and *CS* ≥ 0, *TS* ≥ 0.

*J*

_{ 2 }is the second invariant of the deviatoric stress tensor:

*σ*

_{1}≥ 0) and the minimal principal stress is negative (

*σ*

_{3}≤ 0), whereas the Rankine criterion is used in other situations. The Coulomb-Mohr criterion is formulated as:

*k*represents the ratio between the compressive and tensile strength of the material:

*CS*>

*TS*. After some algebraic manipulation, the safety factor for this criterion can be written, for ductile materials (considered ductile if

*TS*>

*CS*/2), as (see [14]):

*I*

_{ 1 }is the first invariant of the stress tensor:

*k*= 1). For brittle materials (

*TS*≤

*CS*/2), the Christensen criterion includes an additional condition for failure under tensile state:

To compare these criteria, a hypothetical brittle material with TS = 100 MPa and CS = 300 MPa, which is in the range of some brittle dental materials, was considered and the different criteria were compared in a plane stress state.

Three different finite element models were developed in this work to analyse the effect of failure criteria in the FEM results interpretation and to compare DTT and FT for obtaining material properties to be used for these criteria. The CosmosWorks module of the SolidWorks CAD/CAE system (Dassault Systèmes SolidWorks Corp., Concord, MA, USA) and Nastran (MSC.Software Corporation, Santa Ana, CA, USA), were used to solve the models.

^{2}on the palatal side of the tooth, near the incisal edge. This load was applied with an angle of 50° to the radicular axis, in the vestibular direction, as shown in Figure 1, to simulate real biting forces. The analysis was carried out using the finite element analysis software application MSC-Patran-Nastran. Similar models of endodontic restorations were used by the authors in previous works [7, 12] with results that agreed well with the experimental data, thus confirming the fidelity of the model. Once the results of this model had been obtained, different failure criteria (VM, R, CM, MM, C) were applied to every element in the model to obtain the safety factor and the failure point predicted with each criterion. Table 2 shows the TS and CS considered for the different materials.

Material properties of the restored tooth model

Component (Material) | Elastic Modulus (GPa) | Poisson coefficient | Reference |
---|---|---|---|

Root (dentine) | 18.6 | 0.31 | |

Gutta-percha | 0.00069 | 0.45 | |

Periodontal ligament | 0.0689 | 0.45 | |

Cortical bone | 13.7 | 0.30 | |

Trabecular bone | 1.37 | 0.30 | |

Post cement (resin cement) | 18.6 | 0.30 | Coltène Whaledent |

Core (resin composite) | 7.786 | 0.30 | [34] |

Crown (porcelain) | 120 | 0.28 | [4] |

Post (stainless steel) | 207 | 0.30 | Coltène Whaledent |

CS and TS of materials, used for failure theories

*t*) were analysed to study the effect of the diameter-to-thickness ratio, which was varied in previous works [23, 29, 33]. The material properties used for the specimen in the model simulate properties of ParaCore composite resin [34]: elastic modulus E = 7786 MPa and Poisson's ratio ν = 0.3. For the upper and lower compression platens the material properties of steel were considered: E = 206GPa, ν = 0.29.

^{th}of the cylindrical specimen and adding the consequent symmetry constraints (see Figure 2b). The mesh in the specimen was refined progressively towards the contact area. The load, P, was uniformly distributed on the upper plane of the compression platen and a contact condition between the compression platen and the disc was included in the model. The magnitude of the load P in each model was selected as a function of disc thickness (Table 3) to obtain a DTS of 45 MPa, a value in the range of the reported strength of ParaCore resin composite [34, 35]. The DTS value is calculated as the tensile stress in the x-direction in the disc diameter given by x = 0, z = 0, assuming plane stress and a point load [36]:

Load values for DTT models as a function of disc thickness

t (mm) | 1 | 2 | 3 | 4 | 5 | 6 |
---|---|---|---|---|---|---|

Load (N) | 424 | 848 | 1272 | 1696 | 2120 | 2544 |

where P is the failure load and *t* the disc thickness.

where L is the distance between supports, and B and H the width and height of the specimen section, respectively.

Figure 3b shows the mesh of the FEM representing only a quarter of the specimen, taking advantage of the inherent symmetries. A refined mesh was used near the centre of the specimen. Contact conditions between the anvils and the specimen were used in the model.

FE models for DTT and FT were meshed and solved using CosmosWorks.

## Results

*σ*

_{ 2 }= 0) in a plot of maximum principal stress

*σ*

_{ 1 }against minimum principal stress

*σ*

_{ 3 }. Points inside the closed line of each criterion are safe points and points outside the line will fail under this load combination for the corresponding criterion. The VM criterion, typical for ductile materials, presents quite different results compared to other criteria, especially with negative principal stresses (3rd quadrant of the plot). Typical criteria for brittle materials, such as CM and MM, are equivalent in the 1st and 3rd quadrant and similar in the 4th quadrant. The C criterion, used for a brittle material (Eq. 9), is very similar to the MM criterion in the 4th quadrant, but quite different in the 1st and 3rd ones, being more restrictive for positive principal stresses (tension) and less for negative principal stresses (compression). From the comparison, it is clear that in brittle materials, with CS greater than TS, the VM criterion would produce very different results to CM or MM.

Safety Factor and principal stresses (in brackets, MPa) at the most critical point for each component

Cement | Dentine | Post | Crown | Core | |
---|---|---|---|---|---|

VM | 3.96 (-2.3,-4.9,-30.2) | 2.00 (57.6,7.2,4.0) | 8.98 (2.0,-7.2,-161.2) | 1.69 (-4.6,-12.2,-80.8) | 7.76 (-3.0,-4.9,-15.2) |

R | 4.30 (24.6,10.8,1.3) | 1.55 (66.9,23.4,20.1) | 8.71 (-3.2,-10.7,-163.9) | 1.79 (-10.6,-39.6,-91.3) | 8.65 (10.2,2.9,-1.1) |

CM | 4.30 (24.6,10.8,1.3) | 1.55 (66.9,23.4,20.1) | 8.71 (-3.2,-10.7,-163.9) | 1.78 (58.7,20.1,-12.8) | 8.30 (10.2,2.9,-1.1) |

MM | 4.30 (24.6,10.8,1.3) | 1.55 (66.9,23.4,20.1) | 8.71 (-3.2,-10.7,-163.9) | 1.79 (-10.6,-39.6,-91.3) | 8.65 (10.2,2.9,-1.1) |

C | 3.89 (24.6,10.8,1.3) | 1.30 (66.9,23.4,20.1) | 8.98 (2.0,-7.2,-161.2) | 1.97 (58.7,20.1,-12.8) | 8.11 (10.2,2.9,-1.1) |

Figure 1 shows the approximate position of these critical points in each component for the different criteria in the model of the restored tooth with ferrule. Big squares indicate the area for failure initiation of the system predicted by VM (in the crown) and by the rest of criteria (in dentine, in the cervical area under tensile stresses). Results show that the VM criterion predicts different failure positions in brittle components (core, root, cement) compared to the rest of the criteria. As noted before, the C criterion agrees with VM in the post and with other criteria for the brittle components with the exception of the crown, where MM and R predict the lowest SF near the load application area. A more detailed analysis of the results in the crown showed that the SF for this component is similar in the loading area and on the lingual side of the cervical area, where C and CM predict the failure, thereby indicating that both are critical areas for this component. Similar values of the SF were also observed with the VM criterion on the vestibular side of the cervical area and near the loading area.

*z*=

*t*/2. Stresses in the y-direction are compressive, and they are high compared to tensile stresses in the x-direction. Stresses in the z-direction are small except in the load application areas. Figure 5 also shows the areas where the different criteria predict failure initiation in the DTT. The C criterion predicts initiation in the area with greater tensile stress, while other criteria predict initiation near the loading area as a consequence of compressive stresses.

*σ*

_{ x }, along the line defined by

*z = t/2, x = 0, y*= [0,

*D*/2] for the 6 cylindrical specimens of different thicknesses and the theoretical result obtained with the plane stress hypothesis. As seen, the maximum value of

*σ*

_{ x }increases with disc thickness. As expected, the deviation from the plane stress theoretical constant value (45 MPa) increases with disc thickness. Actually, the deviation from the theoretical value is large, even for the thinner discs, when

*y*tends to

*D/2*.

The stress state (σ_{3} vs. σ_{1}) of the critical points of the specimen for the DTT (*t* = 3 mm) and the FT predicted by each criterion compared with the failure lines for these criteria with TS = 100 MPa, CS = 300 MPa is shown in Figure 4. It can be observed that failure with FT, except for the VM criterion, is presented for a stress state with near uniaxial tensile stress in the inferior part of the specimen, whereas a more complex stress state is obtained with DTT regardless of the failure criterion considered.

## Discussion

The use of FEM to simulate dental restorations has increased considerably in the recent years, but a clear and correct procedure to interpret the results is needed to obtain valid conclusions. Complex stress states are present at the different points of the restoration requiring the use of failure criteria to determine whether these points will fail under this stress combination. Two main factors affect the correct interpretation of the results: the selection of the failure criterion and the values of TS and CS required for formulating this criterion.

Referring to the first factor, the results of the present work indicate that using the VM criterion is not adequate to interpret results in brittle components because this criterion is based only on TS. This conclusion is reinforced by the fact that, as has been shown in the results section for the restored tooth simulation, the VM criterion predicts failure at different locations compared to other criteria based on two properties (TS and CS) that are more adequate for brittle materials. A number of previous studies simulating endodontic restorations have interpreted the results based on the VM stress [4–6, 8, 12, 13, 16]. It can be concluded that some of these results should be taken with caution. The Christensen criterion has the advantage of managing both ductile and brittle materials with quite the same formulation, and the results of the present work indicate that the use of this criterion in the simulation of the restored tooth produces equivalent results to VM for ductile components and to CM and MM for brittle components. From the present results the authors recommend the use of this criterion for interpreting FEM results in dental restorations.

The prevalent use of the VM criterion in previous works is probably due to the fact that this is the usual criterion in the majority of engineering calculations and, also for this reason, it is incorporated as the default criterion in most commercial FE packages. The VM criterion makes it possible to perform a simple comparison between an equivalent stress and the tensile strength of the material, but it is only correct for ductile materials. The Christensen criterion has been presented quite recently in the literature [21], which explains why it is not present in commercial FE programs. For the same reason, it is absent in previous FE works on Endodontics. The use of this criterion involves some post-processing with the principal stresses and the TS and CS of the different materials. In any case, if it is not possible to use the C criterion, other long-established brittle criteria, such as CM or MM, are recommended instead of VM for brittle materials.

The second important factor for interpreting FEM results is the definition of material properties TS and CS. Obviously, a proper application of a failure criterion needs a sufficiently accurate value of TS and CS. Usually, obtaining an accurate value of CS is not problematic as it can be obtained from a simple compressive test. Dental materials manufacturers normally supply this data. In contrast, obtaining an accurate value of TS is not always easy. A direct tensile stress test is not suitable for brittle materials, and hence, tensile strength is commonly obtained from indirect tests like DTT or FT.

As for DTT two main assumptions must be made to use the DTS value obtained with Eq. 10 as an estimation of TS. First, it is necessary to assume a plane stress and point load to obtain Eq. 10 [36], and second it is necessary to assume failure initiation in the loading diameter and to neglect the effect of compressive stresses that are present in the disc.

The first assumption of the plane stress hypothesis will be satisfactory only for very thin specimen discs, *t/D*<< 1. Figure 6 shows that the maximum tensile stress value for each case goes away from the theoretical plane stress value as relation *t/D* increases. Only when *t* = 1 mm (*t/D = 0.17*) will the maximum tensile stress value obtained by FEA (44.83 MPa) agree with the theoretical value (45 MPa). However, if *t* = 3 mm (*t/D = 0.5)*, the maximum tensile stress (77.0 MPa) is far from the expected value and for thicker discs disagreement keeps growing. However, values of 0.5 for the thickness-to-diameter ratio are usual in the literature [23, 26, 27, 37], probably to avoid buckling, and even greater values are used in some works, such as 0.8 [28] or 1.5 [29].

The second assumption is also difficult to justify. Figure 4 and Figure 5 show that the predicted failure initiation point is dependent on the failure criterion considered and that compressive stress is high for any of these possible failure points and cannot be neglected. For plane stress, compressive stress in the disc centre is equal to three times the tensile stress at this point, and this stress increases moving in the loading diameter towards the load application point, similar to result obtained with FEA, as shown in Figure 5. Neglecting this compressive stresses is equivalent to implicitly considering a failure criterion, not supported in the literature, given by max{*σ*
_{1}, *σ*
_{2}, *σ*
_{3}} ≤ *TS*. From the results shown in Figure 4, it can be concluded that failure in DTT is related to both tensile and compressive strengths, so the result of this test cannot be used to estimate TS. The situation is quite different for estimating TS from FS obtained with a FT. The FS value is obtained as the maximum tensile stress obtained in a flexural test for a simply supported beam (Eq. 11). To correctly apply Eq. 11, the cross section dimensions of the specimen must be much smaller than its longitudinal dimensions. The ISO 4049 standard defines appropriate test dimensions. FEA results for FT (see Figure 7) show good agreement between the *σ*
_{
z
} |_{max} expected value (90MPa) and the FEA value (85.3MPa). Although high compression values appear in the contacts between the specimen and the anvils, that does not seem to be relevant for the flexural test. Figure 4 and Figure 7 show that the failure initiation point is in the part of the beam section under tensile stress, with a stress state near to uniaxial. Moreover, in this case all the failure criteria except Von Mises (not valid for brittle materials) predict failure at the same point.

Some works have reported differences between DTS and FS results for the same brittle material [23, 29]. Generally, the FS value is greater than DTS. Our simulations confirm this observation. Figure 4 shows that, assuming the Christensen failure criterion, for a material with TS = 100 MPa and FS = 300 MPa, the DTS value will be lower than 45 MPa and the FS will be near 100 MPa.

From previous analyses, it can be concluded that FS is a good estimation for TS in brittle materials and can be used to interpret FEA results, whereas the DTS value is not a good option because is not clearly correlated to TS. Comparison of in vitro DTS of a material with tensile stresses experienced by a component of this material in a FEA, to assess a possible failure, as was done in previous studies [31], cannot be considered correct from the results of this study.

The results of the FE simulation of the endodontic restoration (Figure 1) also confirmed the problems with the use of the VM criterion in brittle materials, because this criterion predicts failure initiation points different to those observed with other criteria that are better suited for use with brittle materials. All the criteria other than the VM predicted the lowest SF in dentine, close to the interface with the crown, on the lingual side of the cervical area. This area is subject to high tensile stress, thus causing fracture of the dentine or the crown or loss of adhesion at the interface between crown and dentine, as has been observed in previous *in vitro* studies [40, 41].

The present study has some limitations, as it considers isotropic linear materials in the restored tooth model. This assumption is common for most simulations, although some materials present some anisotropic behaviour, such as dentine or some composite materials with fillers. Moreover, some components, such as the PDL, introduce non-linear behaviour into the biomechanics of the restored tooth system and this effect is not included in our model, which is linear. Failure analysis for orthotropic or anisotropic materials is not dealt with in the present work. The failure analysis in these materials requires the use of more complex failure criteria [19] and material strength data in different directions are necessary.

## Conclusions

The following conclusions can be drawn from the present study related to the interpretation of finite element results in simulations of dental restorations:

In addressing the possible failure of the restored system, two main factors should be considered: the strength of the different materials involved (tensile strength and compressive strength) and the failure criterion to be used for each material.

The Von Mises criterion is a good option for ductile materials with equal tensile and compressive strength, but it fails with brittle materials. From the results of the present study we recommend the use of the Christensen criterion, which is valid for brittle materials and is coincident with Von Mises for ductile materials.

Flexural strength is a good estimation for tensile strength used in failure criteria. Diametral tensile strength should not be used in this context because failure under this test is related to both tensile and compressive strengths of the material.

## Notes

## Declarations

### Acknowledgements and Funding

We acknowledge to our colleague Dr. Joaquin L. Sancho-Bru its support in the initial conception of the present work. This work was supported by both the Spanish Government and the European Union (FEDER funds) through Project DPI2006-13432.

## Authors’ Affiliations

## References

- Christensen GJ:
**Posts and cores: state of the art.***J Am Dent Assoc*1998,**129:**96–97.View ArticleGoogle Scholar - Davy DT, Dilley GL, Krejci RF:
**Determination of stress patterns in root-filled teeth incorporating various dowel designs.***J Dent Res*1981,**60:**1301–1310. 10.1177/00220345810600070301View ArticleGoogle Scholar - Holmes DC, Diaz-Arnold AM, Leary JM:
**Influence of post dimension on stress distribution in dentin.***J Prosthet Dent*1996,**75:**140–147. 10.1016/S0022-3913(96)90090-6View ArticleGoogle Scholar - Pegoretti A, Fambri L, Zappini G, Bianchetti M:
**Finite element analysis of a glass fibre reinforced composite endodontic post.***Biomaterials*2002,**23:**2667–2682. 10.1016/S0142-9612(01)00407-0View ArticleGoogle Scholar - Asmussen E, Peutzfeldt A, Sahafi A:
**Finite element analysis of stresses in endodontically treated, dowel-restored teeth.***J Prosthet Dent*2005,**94:**321–329. 10.1016/j.prosdent.2005.07.003View ArticleGoogle Scholar - Genovese K, Lamberti L, Pappalettere C:
**Finite element analysis of a new customized composite post system for endodontically treated teeth.***J Biomech*2005,**38:**2375–2389. 10.1016/j.jbiomech.2004.10.009View ArticleGoogle Scholar - Barjau-Escribano A, Sancho-Bru JL, Forner-Navarro L, Rodríguez-Cervantes PJ, Perez-Gonzalez A, Sanchez-Marin FT:
**Influence of prefabricated post material on restored teeth: fracture strength and stress distribution.***Oper Dent*2006,**31:**47–54. 10.2341/04-169View ArticleGoogle Scholar - Boschian-Pest L, Guidotti S, Pietrabissa R, Gagliani M:
**Stress distribution in a post-restored tooth using the three-dimensional finite element method.***J Oral Rehabil*2006,**33:**690–697. 10.1111/j.1365-2842.2006.01538.xView ArticleGoogle Scholar - Sorrentino R, Aversa R, Ferro V, Auriemma T, Zarone F, Ferrari M,
*et al*.:**Three-dimensional finite element analysis of strain and stress distributions in endodontically treated maxillary central incisors restored with different post, core and crown materials.***Dent Mater*2007,**23:**983–993. 10.1016/j.dental.2006.08.006View ArticleGoogle Scholar - Rodríguez-Cervantes PJ, Sancho-Bru JL, Barjau-Escribano A, Forner-Navarro L, Pérez-González A, Sánchez-Marín FT:
**Influence of prefabricated post dimensions on restored maxillary central incisors.***J Oral Rehabil*2007,**34:**141–152. 10.1111/j.1365-2842.2006.01720.xView ArticleGoogle Scholar - Ferrari M, Sorrentino R, Zarone F, Apicella D, Aversa R, Apicella A:
**Non-linear viscoelastic finite element analysis of the effect of the length of glass fiber posts on the biomechanical behaviour of directly restored incisors and surrounding alveolar bone.***Dent Mater*2008,**27:**485–498. 10.4012/dmj.27.485View ArticleGoogle Scholar - Gonzalez-Lluch C, Rodríguez-Cervantes PJ, Sancho-Bru JL, Perez-Gonzalez A, Barjau-Escribano A, Vergara-Monedero M,
*et al*.:**Influence of material and diameter of pre-fabricated posts on maxillary central incisors restored with crown.***J Oral Rehabil*2009,**36:**737–747. 10.1111/j.1365-2842.2009.01989.xView ArticleGoogle Scholar - Hsu ML, Chen CS, Chen BJ, Huang HH, Chang CL:
**Effects of post materials and length on the stress distribution of endodontically treated maxillary central incisors: a 3D finite element analysis.***J Oral Rehabil*2009,**36:**821–830. 10.1111/j.1365-2842.2009.02000.xView ArticleGoogle Scholar - De Groot R, Peters MC, De Haan YM, Dop GJ, Plasschaert AJ:
**Failure stress criteria for composite resin.***J Dent Res*1987,**66:**1748–1752. 10.1177/00220345870660121001View ArticleGoogle Scholar - Craig R, Powers JM:
*Restorative Dental Materials.*11th edition. St Louis: Mosby; 2002.Google Scholar - Yaman SD, Karacaer O, Sahin M:
**Stress distribution of post-core applications in maxillary central incisors.***J Biomater Appl*2004,**18:**163–177. 10.1177/0885328204034745View ArticleGoogle Scholar - Ichim I, Kuzmanovic DV, Love RM:
**A finite element analysis of ferrule design on restoration resistance and distribution of stress within a root.***Int Endod J*2006,**39:**443–452. 10.1111/j.1365-2591.2006.01085.xView ArticleGoogle Scholar - Nakamura T, Ohyama T, Waki T, Kinuta S, Wakabayashi K, Mutobe Y,
*et al*.:**Stress analysis of endodontically treated anterior teeth restored with different types of post material.***Dent Mater J*2006,**25:**145–150. 10.4012/dmj.25.145View ArticleGoogle Scholar - Dejak B, Mlotkowski A, Romanowicz M:
**Strength estimation of different designs of ceramic inlays and onlays in molars based on the Tsai-Wu failure criterion.***J Prosthet Dent*2007,**98:**89–100. 10.1016/S0022-3913(07)60042-0View ArticleGoogle Scholar - Williams JG:
*Stress Analysis of Polymers.*Halsted press, New York; 1973.Google Scholar - Christensen RM:
**A comparative evaluation of three isotropic, two property failure theories.***J Appl Mech*2006,**73:**852–859. 10.1115/1.2173007View ArticleMATHGoogle Scholar - Ban S, Anusavice KJ:
**Influence of test method on failure stress of brittle dental materials.***J Dent Res*1990,**69:**1791–1799. 10.1177/00220345900690120201View ArticleGoogle Scholar - Xie D, Brantley WA, Culbertson BM, Wang G:
**Mechanical properties and microstructures of glass-ionomer cements.***Dent Mater*2000,**16:**129–138. 10.1016/S0109-5641(99)00093-7View ArticleGoogle Scholar - Hondrum SO:
**Storage stability of dental luting agents.***J Prosthet Dent*1999,**81:**464–468. 10.1016/S0022-3913(99)80015-8View ArticleGoogle Scholar - Probster L, Geis-Gerstorfer J, Kirchner E, Kanjantra P:
**In vitro evaluation of a glass-ceramic restorative material.***J Oral Rehabil*1997,**24:**636–645. 10.1046/j.1365-2842.1997.00560.xView ArticleGoogle Scholar - Cefaly DF, Valarelli FP, Seabra BG, Mondelli RF, Navarro MF:
**Effect of time on the diametral tensile strength of resin-modified restorative glass ionomer cements and compomer.***Braz Dent J*2001,**12:**201–204.Google Scholar - Coelho Santos G Jr, El-Mowafy O, Rubo JH:
**Diametral tensile strength of a resin composite core with nonmetallic prefabricated posts: an in vitro study.***J Prosthet Dent*2004,**91:**335–341. 10.1016/j.prosdent.2004.01.017View ArticleGoogle Scholar - Nakamura T, Ohyama T, Imanishi A, Nakamura T, Ishigaki S:
**Fracture resistance of pressable glass-ceramic fixed partial dentures.***J Oral Rehabil*2002,**29:**951–955. 10.1046/j.1365-2842.2002.00929.xView ArticleGoogle Scholar - Della Bona A, Benetti P, Borba M, Cecchetti D:
**Flexural and diametral tensile strength of composite resins.***Braz Oral Res*2008,**22:**84–89. 10.1590/S1806-83242008000100015View ArticleGoogle Scholar - De Jager N, de Kler M, van der Zel JM:
**The influence of different core material on the FEA-determined stress distribution in dental crowns.***Dent Mater*2006,**22:**234–242. 10.1016/j.dental.2005.04.034View ArticleGoogle Scholar - Imanishi A, Nakamura T, Ohyama T, Nakamura T:
**3-D Finite element analysis of all-ceramic posterior crowns.***J Oral Rehabil*2003,**30:**818–822. 10.1046/j.1365-2842.2003.01123.xView ArticleGoogle Scholar - Shigley JE, Mischke CR:
*Diseño En Ingeniería Mecánica.*México: MCGraw-Hill; 2002.Google Scholar - Casselli DS, Worschech CC, Paulillo LA, Dias CT:
**Diametral tensile strength of composite resins submitted to different activation techniques.***Braz Oral Res*2006,**20:**214–218.View ArticleGoogle Scholar - Dodiuk-Kenig H, Lizenboim K, Eppelbaum I, Zalsman B, Kenig S:
**The effect of hyper-branched polymers on the properties of dental composites and adhesives.***J Adhes Sci Tech*2004,**18:**1723–1737. 10.1163/1568561042708304View ArticleGoogle Scholar - Freitas AP, Jumaily S, Santos-Junior GC, Rizkalla A:
*Diametral Tensile Strength and Knoop Hardness of Commercial Core Materials.*IADR 86th General Session & Exhibition, Toronto; 2008.Google Scholar - Jonsén P, Häggblad HA, Sommer K:
**Tensile strength and fracture energy of pressed metal powder by diametral compression test.***Powder Technol*2007,**176:**148–155. 10.1016/j.powtec.2007.02.030View ArticleGoogle Scholar - Brosh T, Ganor Y, Belov I, Pilo R:
**Analysis of strength properties of light-cured resin composites.***Dent Mater*1999,**15:**174–179. 10.1016/S0109-5641(99)00029-9View ArticleGoogle Scholar - Eskitascioglu G, Usumez A, Sevimay M, Soykan E, Unsal E:
**The influence of occlusal loading location on stresses transferred to implant-supported prostheses and supporting bone: A three-dimensional finite element study.***J Prosthet Dent*2004,**91:**144–150. 10.1016/j.prosdent.2003.10.018View ArticleGoogle Scholar - Plotino G, Grande NM, Bedini R, Pameijer CH, Somma F:
**Flexural properties of endodontic posts and human root dentin.***Dent Mater*2007,**23:**1129–1135. 10.1016/j.dental.2006.06.047View ArticleGoogle Scholar - Raygot CG, Chai J, Jameson L:
**Fracture resistance and primary failure mode of endodontically treated teeth restored with a carbon fiber-reinforced resin post system in vitro.***Int J. Prosthodont*2001,**14:**141–145.Google Scholar - Sidoli EG, King PA, Setchell DJ:
**An in vitro evaluation of a carbon-fiber based post and core system.***J Prosthet Dent*1997,**78:**5–9. 10.1016/S0022-3913(97)70080-5View ArticleGoogle Scholar

## Copyright

This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.